Download presentation

Presentation is loading. Please wait.

Published byValerie Trepp Modified about 1 year ago

1
Connie B. Roth, Chris A. Murray and John R. Dutcher Department of Physics University of Guelph Guelph, Ontario, Canada N1G 2W1 COMPLEX FLOW OF NANOCONFINED POLYMERS

2
instabilities in freely-standing liquid films hole growth in freely-standing PS films – ideal geometry for probing complex flow – shear thinning – convective constraint release relaxation mechanism – hole growth occurs for T comparable to T g bulk hole growth in freely-standing PS/PI/PS trilayer films – holes in central PI layer summary & conclusions OUTLINE

3
CURRENT PROJECTS POLYMERS BIOPOLYMERS BACTERIAL CELLS molecular mobility – glass transition & hole growth instabilities & pattern formation biodegradable polymers polypeptides & proteins – lipid membranes & polymer brushes bacterial adhesion & physical properties of bacteria & biofilms

4
to measure structure, dynamics, interaction forces, molecular conformations, adsorption kinetics, we use – atomic force microscopy – ellipsometry – surface plasmon resonance – quartz crystal microbalance – optical tweezers – TIRF – infrared techniques (PM-IRRAS, ATR-FTIR) – surface circular dichroism – TEM – differential pressure techniques SURFACE-SENSITIVE PROBES

5
THIN LIQUID FILMS thin liquid films occur in everyday life – adhesives (superglue) – lubricants (on cornea of eye, engine piston) – spray coatings (paint, herbicides, fibers) – printing (ink on transparency or tape) – soap bubbles & films – foams (shaving cream, cappuccino) – water films (water spotting, hydroplaning) stability desirable/ essential stability undesirable

6
hole radius grows linearly with time [Taylor, Proc. Roy. Soc. (1959)] [Culick, J. Appl. Phys. (1960)] t – fluid collects in a rim – rest of film undisturbed R t HOLE GROWTH IN NON-VISCOUS FILMS

7
h POLYMER MOLECULES polymers are complex molecules – different length scales ranging from segment size to overall chain size R EE ~ M w 0.5 – different time scales ranging from segmental relaxation to diffusion of entire molecules R EE – effect of confinement in thin films – changes in conformation & dynamics

8
hole radius grows exponentially with time [Debrégeas et al., PRL (1995)] t – no rim – film thickens uniformly HOLE GROWTH IN VISCOUS FILMS

9
FREELY-STANDING FILM PREPARATION spincoat polymer solution onto mica substrate anneal film under vacuum transfer film onto water surface capture film on holder containing 4 mm diameter hole high molecular weight, monodisperse polymers dissolved in good solvents

10
– plug flow – driven by surface tension – polymer chains become aligned near edge of hole HOLE GROWTH IN POLYMER FILMS 10 m at edge of hole; into rest of film

11
optical microscopy of freely- standing polystyrene films –M w = 717k –96 nm < h < 372 nm –T = 115 o C (T g bulk = 97 o C) –exponential hole growth –decrease in viscosity for increasing strain rate –consistent with shear thinning [Dalnoki-Veress et al., PRE 59, 2153 (1999)] PREVIOUS HOLE GROWTH IN PS FILMS

12
SHEAR THINNING OF POLYMERS decrease in viscosity with increasing shear strain rate – shear thinning only observed for entangled polymers [Peterlin, Adv. Macromol. Chem. 1, 225 (1968)] – is M w -independent in nonlinear regime [Stratton, J. Colloid Interf. Sci. 22, 517 (1966)] log 00 log PS of diff M w

13
SHEAR THINNING IN FREELY-STANDING PS FILMS use growth time to obtain viscosity at edge of hole plot / 0 versus reduced shear strain rate results consistent with viscous flow in presence of shear thinning different T, M w and h optical microscopy + differential pressure experiment [Roth & Dutcher, PRE 72, (2005)]

14
FLOW AT SUCH LOW TEMPERATURES? in bulk, viscosity 0 ~ Pas at T ~ T g – expect both viscous and elastic effects important – late stage hole growth is well-described by viscous flow previous studies of crazing of PS films [Berger & Kramer, Macro (1987)] – chain scission at low temperatures – chain disentanglement at strain rates & higher temps – for M w = 1800k: T > 70 o C for ˙ = 4.1 x s -1 T > 90 o C for ˙ ~ s -1 comparable strain rates & temps for hole growth 1.5 x s -1 < ˙ < 2 x s -1 for 101 o C < T < 117 o C

15
TRANSITION IN HOLE GROWTH measure R(t) for single hole using optical microscopy – linear growth at early times – velocity v – exponential growth at late times – growth time – range of times for linear growth decreases with – increasing T – decreasing M w R = R o + v t R = R o exp(t / ) PS M w = 2240k, h = 79 nm at T = 103 o C [Roth et al., PRE 72, (2005)]

16
TRANSIENT BEHAVIOR scale axes: ln[R(t)/R( )] vs t/ – data sets coincide for t > isolate transient – single exponential decay time 1 M w = 717k h = 125 nm

17
TRANSITION IN HOLE GROWTH measure R(t) for single hole using optical microscopy – linear growth at early times – velocity v – exponential growth at late times – growth time – range of times for linear growth decreases with – increasing T – decreasing M w R = R o + v t R = R o exp(t / ) PS M w = 2240k, h = 79 nm at T = 103 o C [Roth et al., PRE 72, (2005)]

18
TRANSIENT BEHAVIOR scale axes: ln[R(t)/R( )] vs t/ – data sets coincide for t > isolate transient – single exponential decay time 1 refer t to t 0 for which R(t 0 ) = 0 – overlap of data – decay time 1 scales with M w = 717k h = 125 nm

19
FITTING FUNCTION FOR R(t) empirically, R(t) data for all times well fit by – equivalent to time-dependent viscosity (t) – described by a three-component spring & dashpot model where is viscosity for t >> 1 single relaxation time E

20
FITS TO R(t) DATA 3 fitting parameters: R 0 value at start of measurements (t = 0) exponential hole growth time 1 longest relaxation time M w = 717 × 10 3 h = 90 nm

21
RELATIONSHIP BETWEEN AND 1 and 1 have similar temperature dependence with 1 ~ /2 data 1 data / 1 = 2.2 ± 1.4]

22
TUBE MODEL FOR POLYMER DYNAMICS low shear rate ˙ < d -1 reptation + contour length fluctuations (CLF) intermediate shear rate d -1 < ˙ < R -1 convective constraint release (CCR) high shear rate R -1 < ˙ chain stretch [Graham, Likhtman, McLeish, and Milner, J. Rheol (2003)] d Reptation time R Rouse time Hole growth at T = 101 o C d -1 ~ s -1 R -1 ~ s -1 ˙ ~ s -1 hole growth at lowest temperatures occurs in the intermediate to high shear rate regimes – relaxation via CCR (no rotation in flow) – since ˙ = 2 / expect 1 ~ ˙ -1 ~ / 2 → data consistent with CCR

23
DIFFERENTIAL PRESSURE EXPERIMENT differential pressure experiment [Roth et al., RSI 74, 2796 (2003); Roth & Dutcher, PRE 72, (2005)] – maintain pressure difference across PS film – track piston position as a function of time PS, M w = 2240k, h = 69 nm, T = 98 o C

24
DPE RESULTS FOR FREELY-STANDING PS FILMS temperature dependence of hole growth time – M w = 717k, 2240k – 51 nm < h < 98 nm – 92 o C < T < 105 o C – consistent with shear thinning – despite large differences in T g, onset temperature for hole formation is comparable to T g bulk for all films [Roth et al., RSI 74, 2796 (2003); Roth & Dutcher, PRE 72, (2005)]

25
FREELY-STANDING TRILAYER FILMS trilayer films with central fluid layer and solid capping layers – periodic lateral morphology forms upon heating due to amplification of thermal fluctuations PS/PI/PS [K. Dalnoki-Veress et al., PRL 82, 1486 (1999)] [C.A. Murray et al., PRE 69, (2004)]

26
HOLE GROWTH IN PS/PI/PS TRILAYERS hole growth in PS freely-standing films – uniform thickening of films – absence of rim at edge of hole hole growth in PS/PI/PS freely-standing films – holes form & grow in central PI layer – distinct rim at edge of hole

27
HOLE GROWTH IN PS/PI/PS TRILAYERS presence of rim verified using atomic force microscopy (AFM) optical microscopy AFM [C.A. Murray et al. (2006)] h = 50 nm, L = 75 nm

28
HOLE GROWTH IN PS/PI/PS TRILAYERS radius of hole in PI layer measured at fixed temperature T = 110 o C fix PS thickness L vary PI thickness h fix PI thickness h vary PS thickness L [C.A. Murray et al. (2006)]

29
HOLE GROWTH IN PS/PI/PS TRILAYERS relevant factors that determine hole growth in PI layer – surface & PS/PI interfacial energies – bending energy of PS layers – dispersion interaction between the PS/air interfaces – can understand slowing of hole growth with increase in h & L

30
SUMMARY hole growth in freely-standing PS films – two different experiments – shear thinning – convective constraint release – hole growth occurs at temperatures comparable to T g bulk hole growth in fs PS/PI/PS films – qualitatively different hole growth – hole growth in PI determined by PS

Similar presentations

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google